Structural Grades of Timber by Bending and Compression Tests Jorge Branco 1,a, Humberto Varum 2,b and Paulo Cruz 1,c


 Jared Kelly
 1 years ago
 Views:
Transcription
1 Structural Grades of Timber by Bending and Compression Tests Jorge Branco 1,a, Humberto Varum 2,b and Paulo Cruz 1,c 1 DECivil Engineering School, Campus de Azurém, Guimarães, Portugal 2 DECivil, Campus Universitário de Santiago, Aveiro, Portugal a b c Keywords: Timber, structural grades, mechanical tests, bending and compression Abstract. This paper presents the results obtained in a series of tests on Pinus Pinaster Ait. timber specimens, using the pren408:2000, to estimate the local and global Young s modulus and strength both in bending and compression parallel to the grain. The results obtained are compared with the values presented in the Portuguese Nationally Determined Parameters of Eurocode 5, for the quality classes assign by Portuguese Standard NP4305:1994 by visual grading. Introduction The results achieved in any assessment of mechanical properties are function of the testing method adopted. Timber mechanical properties depend of various factors, as for instance: load duration, moisture content, span, depth of the section, etc. Therefore, to accomplish the comparison between the results obtained in different laboratories, a standardization of the test procedure is required. Moreover, with the adoption of limit state design and with the development of both visual and machine stress grading, attention will be increasingly focused on the determination and monitoring of the strength properties and variability of structural grades of timber. The pren408:2000 European Standard specifies laboratory methods for the determination of some physical and mechanical properties in structural sizes. This standard presents test methods for determining the modulus of elasticity, the bending strength and the compression strength in a parallel direction to the grain orientation in structural timber. In addition, the determination of dimensions, moisture content and density are specified. In follow the bending and compression tests procedure adopted by pren408:2000 are described. Bending Test. This test use a piece simply supported with a span of 18 times the depth with the loads points placed on the third of the span, as it is shown in Fig. 1. Small steel plates of length not greater than onehalf of the depth of the test piece may be inserted between the piece and the loading heads supports to minimize local indentation. >h/2 a = 6h 6h 6h F/2 l = 5h F/2 1 >h/2 l = 18h Fig. 1  Test arrangement of the bending test The evaluation of the modulus of elasticity in bending is based on the deformations measured at the centre of a central gauge length of 5 times the depth of the section. This deformation shall be taken as the average of measurements on both faces at the neural axis. w h
2 The local modulus of elasticity in bending (E m,l )is obtained from the follow equation: 2 al1 F E m, l =. (1) 16 I w where F is an increment of load on the straightline portion of the load deformation curve (N), w is the increment of deformation corresponding (mm), a is the distance between a loading position and the nearest support (mm), l 1 is the gauge length (mm) and I is the second moment of area (mm 4 ). Using the deformation value measured at the centre of the span and at the centre of the compression or tension edge we can also calculate the value of the global modulus of elasticity in bending. Thus, the global modulus of elasticity in bending (E m,g ) is obtained from the follow equation: 3 3 l F 3a a E m, g = 3. (2) b h w 4l l where b and h are the width and depth of the cross section (mm), respectively, l is the span (mm). The bending strength is obtained with the continuation of the test just to failure, applying the load with a constant loadinghead movement so adjust that maximum load is reached within (300±120)s. Therefore, the bending strength (f m ) is given by: a Fmax f m =. (3) 2W where F max is the maximum load (N) and W is the section modulus (mm 3 ). Compression Test. In this test, the test piece shall be of full cross section, and shall have a length of 6 times the smaller crosssectional dimension. The end surfaces shall be accurately prepared to ensure that they are plane and parallel to one another and perpendicular to the axis of the piece. The load shall be applied concentrically using spherical seated loading heads permitting the application of a compressive load without inducing bending. Deformation shall be measured over a central gauge length of 4 times the smaller crosssectional dimension of the piece, using two mechanical strain gauges positioned in such way that the eventual effects of distortion shall be minimized. The modulus of elasticity in compression parallel to the grain (E c,0 ) is given as the result of: l F E c = 1, 0. (4) A w where A is the crosssectional area (mm 2 ). The compression strength is obtained with the increment of the load, applied at a constant loadinghead movement so adjusted that maximum load (F max ) is reached within (300±120)s. The compression strength (f c,0 ) is taken as the result of the follow equation: Fmax f c, 0 =. (5) A The mode of fracture and growth characteristics at the fracture section of each test piece shall be reported. Experimental Activity The experimental program is based on Pinus pinaster Ait. specimens classified as belonging to quality class EE in result of a visual strength grading conducted following the National Standard NP 4305:1995 [2]. In both tests kinds conducted, the failure time was register and the moisture content of each specimen was measure with an electronic thermohygrometer for wood. The tests
3 were carried out at the Structural Laboratory of the Civil Engineering Department of the Minho University. Bending Tests. Four beams with a cross section of 80x105 mm 2 and 1.95 m length were evaluated by fourpoints bending tests using a test arrangement following pren 408:2000 (see Fig. 1). A displacement control procedure (0.14 mm/s) with an actuator having a capacity of 100 kn has been used. In each test, apart the registration of the deformations measured at the centre of a central gauge length of 5 times the depth of the section, the deformations at the centre of the span at the centre of the tension side edge were measured. With the deformations values corresponding to the elastic deformation the calculation of the local and global values of the modulus of elasticity in bending were possible. Incrementing the load, it was also possible to obtain the bending strength as it was previously explained (Eq. 3). The bending tests results founded are presented in Table 1. Table 1 Bending tests results Beam Moisture (%) F max (kn) Time (s) E m,l (N/mm 2 ) E m,g (N/mm 2 ) f m (N/mm 2 ) B B B B Mean CoV Like it was expected, the local value for the modulus of elasticity (E m,l ) was always higher than the global value (E m,g ) as no shear deformation is taken into account in first value contrarily to the second. However the pleasants coefficients of variance (CoV) presented by both modulus of elasticity (E m,l = 0.16 and E m,g = 0.11), beam B4 did not reached the bending strength level presented by the others beams. As Fig. 2 show, the maximum load reached by B4 stay quite far from the others results, with direct consequences in the bending strength CoV (0.27). 20 Load (kn) Midspan deformation (mm) Fig. 2 Midspan deformation vs load curves obtained in the bending tests B1 B2 B3 B4 Compression Tests. Four specimens of 80x105x480 mm 3 were used in the compression tests conducted in accordance with the recommendations presented by pren 408:2000. The tests were performed under displacement control with a velocity of 0.01 mm/s using a load cell of 500 kn. Two mechanical strain gauges (one in each the two bigger crosssectional dimensions) were used to measure the deformations and one additional LVDT (Linear Variable Displacement Transducer) was placed in the loading head of the test machine, measuring thereby the grain displacement
4 presented by the specimens. After the moisture content measurement, the specimens were tested with a correct loading head movement (all the failure were reached within 300±120s). Base in the mean values of the deformation measured by the two mechanical strain gauges (in the range of elastic deformation) it was possible to calculated the modulus elasticity (E c,0 ) and with the maximum load value the calculation of the compression strength (f c,0 ). Table 2 shows the compression tests results carried out. Table 2 Compression tests results Specimen Moisture (%) Time (s) F max (kn) E c,0 (N/mm 2 ) f c,0 (N/mm 2 ) S S S S Mean CoV It is clearly show by the results achieved that the compression behaviour of timber is quite heterogeneous. The coefficient of variance presented by the modulus of elasticity and strength round 0.3. This conclusion is confirmed by the observation of the experimental grain displacementload curves presented in Fig. 3. Load (kn) C1 C2 C3 C Grain displacement (mm) Fig. 3 Grain displacement  load curves obtained in the compression tests The Fig. 3 confirm the plastic behaviour recognize to wood under compression parallel to grain and point out a good softening in the grain displacementload curves. Discussion of the Results On the basis of the experimental results, it can be stated the pleasant homogeneity presented by the bending behaviour, especially in terms of elastic modulus. The local modulus of elasticity in bending (E m,l ) presented a CoV equal to 0.11 while the global modulus of elasticity (E m,g ) achieved showed a CoV of In terms of the compression parallel to grain tests results, although the plastic behaviour obtained and the ductile failures achieved, a significant variability was pointed out. Coefficients of variations near of 0.3 were obtained for the elastic modulus and strength. When comparing the experimental results with the values reported in the Portuguese Nationally Determined Parameters of Eurocode 5 (DNA EC5) [3], for the quality class assign in the visual grading performed following NP4305:1995 [2] (Table 3), different conclusions are reached: (1) the bending strength achieved is 21.6% higher than the characteristic value assumed by the National Standard; (2) the mean value obtained for the modulus of elasticity (E m,l ) is 34.2% smaller that the
5 one suggest by DNAEC5; and (3) good agreement between the compression strength value adopted in the DNAEC5 and the experimental results. If the experimental result was MPa, DNAEC5 suggests 24.7 MPa as the characteristics value for the compression strength parallel to the grain. In this standard any value of modulus of elasticity in compression parallel to the grain is presented. Table 3 Mechanical properties of Pinus Pinaster Ait. Class EE [3] Class E m (N/mm 2 ) f m (N/mm 2 ) f c,0 (N/mm 2 ) EE It is important to remember that the values exposed in the DNAEC5 were obtained on specimens free from faults, with nonstructural dimensions and with a moisture content of 12%. It is recognize that the mechanical characterization of wood by means of tests on specimens in small dimension can be inadequate to have reliable and complete information on the structural behaviour of timber elements and structures. For instance, the failure modes obtained in the bending tests conducted are quite different from typical bending failure characteristic of small pieces free from faults, Fig. 4 (a). The existence of knots does not allow the development of the plastic behaviour in the compression side of the cross section (see Fig. 2). Failure append in the tension side and progress rapidly under influence of shear forces without any plastification of the compression side, while the formation of a plastic hinge in the compression side is always obtained in specimens free from faults. In compression, also the existence of faults can determine the failure mode. If in this kind of test the failure mode is more and less constant, is development is always stipulate by the presence of knots, reaction wood, etc., Fig. 4 (b). (a) Bending test B2 (b) Compression test S3 Fig. 4 Failure modes obtained in the experimental work Conclusions With a natural material like wood, so depending of the existence of faults, the mechanical evaluation can not use small specimens free from faults, especially when their presence have the importance showed in this work. Attention has to be moved towards the experimental investigation of the mechanical evaluation of wood elements having structural dimensions and presenting the natural faults recognize to this material. References [1] pren 408:2000: Timber structures Structural timber and glued laminated timber Determination of some physical and mechanical properties, CEN, [2] NP 4305:1995: Structural maritime pine swan timber Visual grading, CT 14 LNEC, [3] NP ENV :1998: Eurocódigo 5  Projecto de estruturas de Madeira. Parte 11: Regras gerais e regras para edifícios. CT 115 LNEC, 1998.
6
Densified Veneer Wood for Notched Joints in Timber Concrete Composite Structures
Densified Veneer Wood for Notched Joints in Timber Concrete Composite Structures 1 Summary Dias, A.M.P.G. (alfgdias@dec.uc.pt) Assistant Professor University of Coimbra CoimbraPortugal Kuilen, J.W.G.,
More informationDEVELOPMENT OF A NEW TEST FOR DETERMINATION OF TENSILE STRENGTH OF CONCRETE BLOCKS
1 th Canadian Masonry Symposium Vancouver, British Columbia, June 5, 013 DEVELOPMENT OF A NEW TEST FOR DETERMINATION OF TENSILE STRENGTH OF CONCRETE BLOCKS Vladimir G. Haach 1, Graça Vasconcelos and Paulo
More informationPin jointed structures are often used because they are simple to design, relatively inexpensive to make, easy to construct, and easy to modify.
4. FORCES in PIN JOINTED STRUCTURES Pin jointed structures are often used because they are simple to design, relatively inexpensive to make, easy to construct, and easy to modify. They can be fixed structures
More informationLOADCARRYING CAPACITY OF AXIALLY LOADED RODS GLUEDIN PERPENDICULAR TO THE GRAIN
LOADCARRYING CAPACITY OF AXIALLY LOADED RODS GLUEDIN PERPENDICULAR TO TE GRAIN Prof. Dr.Ing..J. Blaß, Dipl.Ing. B. Laskewitz Universität Karlsruhe (T), Germany Abstract Gluedin rods have been used
More informationBending Beam. Louisiana State University. Joshua Board
Bending Beam Louisiana State University Joshua Board Table of Contents: Table of Figures:... 4 Purpose... 5 Introduction... 5 Apparatus and Test Procedures... 11 Summary of Data... 14 Discussion of Results...
More informationStrength of Bolted Timber Connections with Steel Side Members
United States Department of Agriculture Forest Service Forest Products Laboratory Research Paper FPLRP513 Strength of Bolted Timber Connections with Steel Side Members T. L. Wilkinson Abstract This study
More informationStructural materials Characteristics, testing, strength evaluation
Budapest University of Technology and Economics Department of Mechanics and Materials of Structures English courses General course /2013 Fundamentals of Structures BMEEPSTG201 Lecture no. 3: Structural
More informationBuilding Project using PostTensioning
Building Project using PostTensioning Paulo Marques 1 Resume Nowadays building flexibility is an aspect to be taken into account at the idealization and project stages. The number of buildings that throughout
More informationLaboratory Weeks 9 10 Theory of Pure Elastic Bending
Laboratory Weeks 9 10 Theory of Pure Elastic Bending Objective To show the use of the Sagital method for finding the Radius of Curvature of a beam, to prove the theory of bending, and find the elastic
More informationNUMERICAL ANALYSIS OF GLULAM BEAMS WITHOUT AND WITH GFRP REINFORCEMENT
10th International Conference on Composite Science and Technology ICCST/10 A.L. Araújo, J.R. Correia, C.M. Mota Soares, et al. (Editors) IDMEC 2015 NUMERICAL ANALYSIS OF GLULAM BEAMS WITHOUT AND WITH GFRP
More informationUnit 48: Structural Behaviour and Detailing for Construction. Chapter 13. Reinforced Concrete Beams
Chapter 13 Reinforced Concrete Beams Concrete is a material strong in its resistance to compression, but very weak indeed in tension. good concrete will safely take a stress upwards of 7 N/mm 2 in compression,
More informationNonLinear Analysis of Bolted Extended EndPlate Steel BeamTo Column Connection Cut Ainul Mardziah Amir,Redzuan Abdullah
NonLinear Analysis of Bolted Extended EndPlate Steel BeamTo Column Connection Cut Ainul Mardziah Amir,Redzuan Abdullah Faculty of Civil Engineering, Universiti Teknologi Malaysia, Malaysia redzuan@utm.my
More informationTensile Testing. Objectives
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
More informationCost Action FP1101 Assessment, Reinforcement and Monitoring of Timber Structures
Cost Action FP1101 Assessment, Reinforcement and Monitoring of Timber Structures Short Term Scientific Mission Report: ASSESSMENT AND DIAGNOSIS OF AN ANCIENT COLLAR TRUSS BY MEANS OF VISUAL GRADING AND
More informationOptimising plate girder design
Optimising plate girder design NSCC29 R. Abspoel 1 1 Division of structural engineering, Delft University of Technology, Delft, The Netherlands ABSTRACT: In the design of steel plate girders a high degree
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationNonlinear Models of Reinforced and Posttensioned Concrete Beams
111 Nonlinear Models of Reinforced and Posttensioned Concrete Beams ABSTRACT P. Fanning Lecturer, Department of Civil Engineering, University College Dublin Earlsfort Terrace, Dublin 2, Ireland. Email:
More informationHardened Concrete. Lecture No. 14
Hardened Concrete Lecture No. 14 Strength of Concrete Strength of concrete is commonly considered its most valuable property, although in many practical cases, other characteristics, such as durability
More informationPLASTIC DEFORMATION AND STRESSSTRAIN CURVES
PLASTIC DEFORMATION AND STRESSSTRAIN CURVES Introduction Background Unit: Plastic Deformation and StressStrain Curves In the last unit we studied the elastic response of materials to externally applied
More informationENGINEERING SCIENCE H1 OUTCOME 1  TUTORIAL 3 BENDING MOMENTS EDEXCEL HNC/D ENGINEERING SCIENCE LEVEL 4 H1 FORMERLY UNIT 21718P
ENGINEERING SCIENCE H1 OUTCOME 1  TUTORIAL 3 BENDING MOMENTS EDEXCEL HNC/D ENGINEERING SCIENCE LEVEL 4 H1 FORMERLY UNIT 21718P This material is duplicated in the Mechanical Principles module H2 and those
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationSTRENGTH OF MATERIALS LABORATORY
STRENGTH OF MATERIALS LABORATORY 1. TESTING OF MATERIALS IN TORSION OBJECTIVE To apply an increasing torque to straight cylindrical specimens of material, to observe the deformation of the specimens, and
More informationTimber Frame Moment Joints with GluedIn Steel Rods  A Designer s Perspective. Mark L Batchelar 1
Timber Frame Moment Joints with GluedIn Steel Rods  A Designer s Perspective Abstract: Mark L Batchelar 1 Significant evidence based on experimental research exists to give designers confidence in the
More informationMSE200 Lecture 7 (CH ) Mechanical Properties I Instructor: Yuntian Zhu Objectives/outcomes: You will learn the following:
MSE200 Lecture 7 (CH. 6.26.4) Mechanical Properties I Instructor: Yuntian Zhu Objectives/outcomes: You will learn the following: Stresses and strains in solids. Normal and shear stresses. Elastic and
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationBEHAVIOUR OF STRUCTURAL INSULATED PANELS (SIPS) UNDER BOTH SHORTTERM AND LONGTERM LOADINGS
Proceedings of the 11th International Conference on Nonconventional Materials and Technologies (NOCMAT 2009) 69 September 2009, Bath, UK BEHAVIOUR OF STRUCTURAL INSULATED PANELS (SIPS) UNDER BOTH SHORTTERM
More informationAdhesion and Viscoelasticity Properties of PVB in Laminated Safety Glass
Adhesion and Viscoelasticity Properties of PVB in Laminated Safety Glass Maurizio FROLI Professor Department of Civil Engineering, Structural Division University of Pisa, Pisa, Italy Maurizio Froli, born
More informationNumerical modelling of shear connection between concrete slab and sheeting deck
7th fib International PhD Symposium in Civil Engineering 2008 September 1013, Universität Stuttgart, Germany Numerical modelling of shear connection between concrete slab and sheeting deck Noémi Seres
More informationStatics and Mechanics of Materials
Statics and Mechanics of Materials Chapter 4 Stress, Strain and Deformation: Axial Loading Objectives: Learn and understand the concepts of internal forces, stresses, and strains Learn and understand the
More informationSPECIFICATIONS, LOADS, AND METHODS OF DESIGN
CHAPTER Structural Steel Design LRFD Method Third Edition SPECIFICATIONS, LOADS, AND METHODS OF DESIGN A. J. Clark School of Engineering Department of Civil and Environmental Engineering Part II Structural
More informationTorsion Testing. Objectives
Laboratory 4 Torsion Testing Objectives Students are required to understand the principles of torsion testing, practice their testing skills and interpreting the experimental results of the provided materials
More informationThe University of Birmingham (Live System)
The University of Birmingham (Live System) Behaviour of Structural Insulated Panels (SIPs) under both shortterm and longterm loadings Yang, Jian; Rungthonkit, Prathan Document Version Author final version
More information1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine Spring 2004 TENSILE TESTING AND STRESS STRAIN PROPERTIES OF STEEL
1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine MIT Spring 2004 Purpose: LABORATORY ASSIGNMENT NUMBER 2 TENSILE TESTING AND STRESS STRAIN PROPERTIES OF STEEL You will learn about:
More informationLocal buckling of plates made of high strength steel
Local buckling of plates made of high strength steel Tapani Halmea, Lauri Huusko b,a, Gary Marquis a, Timo Björk a a Lappeenranta University of Technology, Faculty of Technology Engineering, Lappeenranta,
More informationKINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK. UNIT I STRESS STRAIN DEFORMATION OF SOLIDS PART A (2 Marks)
KINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK SUB CODE/NAME: CE1259 STRENGTH OF MATERIALS YEAR/SEM: II / IV 1. What is Hooke s Law? 2. What are the Elastic Constants?
More informationSTUDY THE EFFECT OF THE VARIATION OF LAYER'S THICKNESS ON THE BENDING CHARACTERISTICS OF THE COMPOSITE BEAM
STUDY THE EFFECT OF THE VARIATION OF LAYER'S THICKNESS ON THE BENDING CHARACTERISTICS OF THE COMPOSITE BEAM Assist. Lecturer Manal Hameed Jasem AlMustansiriya University/College of Eng./Mech. Eng. Depart.
More informationSTRESS GRADES FIGURE 1
STRESS GRADES 300. STRESS GRADES 310. STRESSES ILLUSTRATED 310a. Extreme Fibre in Bending F b and Horizontal Shear  F v In structures, stress grades of lumber may carry loads on spans between supports
More informationσ = F / A o Chapter Outline Introduction Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? and Tension Compression Shear Torsion Elastic deformation Chapter Outline Introduction To understand and describe how materials
More informationDeflection Calculation of RC Beams: Finite Element Software Versus Design Code Methods
Deflection Calculation of RC Beams: Finite Element Software Versus Design Code Methods G. Kaklauskas, Vilnius Gediminas Technical University, 1223 Vilnius, Lithuania (gintaris.kaklauskas@st.vtu.lt) V.
More informationME 105 Mechanical Engineering Laboratory Spring Quarter Tensile Test
ME 105 Mechanical Engineering Lab Page 1 ME 105 Mechanical Engineering Laboratory Spring Quarter 2003 3. Tensile Test Introduction In this lab, you will study the deformation and fracture characteristics
More informationStress Strain Relationships
Stress Strain Relationships Tensile Testing One basic ingredient in the study of the mechanics of deformable bodies is the resistive properties of materials. These properties relate the stresses to the
More informationTimber identified by calling up a specific grade
Grading Production process in the mill prior to packing and shipping Sorting of products into groups with similar characteristics and properties Appearance grade Structural t grade Sorting Criteria  visual
More informationSEISMIC RETROFIT OF UNREINFORCED CLAY BRICK MASONRY WALL USING POLYMERCEMENT MORTAR
SEISMIC RETROFIT OF UNREINFORCED CLAY BRICK MASONRY WALL USING POLYMERCEMENT MORTAR K. Kikuchi 1, M. Kuroki 2, M. Toyodome 3, C. Escobar 4 and Y. Nakano 5 ABSTRACT : 1 Professor, Dept. of Architectural
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationThere are three principle ways a load can be applied:
MATERIALS SCIENCE Concepts of Stress and Strains Stressstrain test is used to determine the mechanical behavior by applying a static load uniformly over a cross section or a surface of a member. The test
More informationFatigue Testing. Objectives
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
More informationWood: Strength and Stiffness
Wood is one of the oldest and bestknown structural materials, and one of the few renewable natural resources. Wood is a desirable material for construction because it requires less energy to produce a
More informationP4 Stress and Strain Dr. A.B. Zavatsky MT07 Lecture 4 Stresses on Inclined Sections
4 Stress and Strain Dr. A.B. Zavatsky MT07 Lecture 4 Stresses on Inclined Sections Shear stress and shear strain. Equality of shear stresses on perpendicular planes. Hooke s law in shear. Normal and shear
More informationVisual grading of large cross section structural timber of Pinus sylvestris L. according to UNE 56544:2007 standard
Visual grading of large cross section structural timber of Pinus sylvestris L. according to UNE 56544:2007 standard MaríaJosé Montero 1, aquel Mateo 2, Guillermo ÍñiguezGonzález 3, Francisco Arriaga
More informationStressStrain Relationship
(Strength of Materials) Dave Morgan StressStrain Relationship p. 1/21 The tension test: StressStrain Relationship p. 2/21 The tension test: Is a common standardised test that can
More informationSection 1: THE TEST CERTIFICATE
Section 1: THE TEST CERTIFICATE The objective of Section 1 is to explain the Metallurgical makeup of the Material Test Certificate. Introduction A material test certificate is used to report the chemical
More informationEFFECTIVE BENDING CAPACITY OF DOWELTYPE FASTENERS
EFFECTIVE BENDING CAPACITY OF DOWELTYPE FASTENERS Hans Joachim Blass 1), Adriane Bienhaus 1) and Volker Krämer 1) 1) Lehrstuhl für Ingenieurholzbau und Baukonstruktionen, University of Karlsruhe, Germany
More informationEMPA, Swiss Federal Laboratories for Materials Science and Technology
Notched Beams Robert Widmann Image: Robert Butler EMPA, Swiss Federal Laboratories for Materials Science and Technology With strong contributions from: Robert Jockwer ETHZ, Swiss Federal Institute of Technology,
More informationComparison of typical 3D printing materials [1]
Comparison of typical 3D printing materials [1] ABS Its strength, flexibility, machinability, and higher temperature resistance make it often a preferred plastic for engineers, and professional applications.
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationReinforced Concrete Design SHEAR IN BEAMS
CHAPTER Reinforced Concrete Design Fifth Edition SHEAR IN BEAMS A. J. Clark School of Engineering Department of Civil and Environmental Engineering Part I Concrete Design and Analysis 4a FALL 2002 By Dr.
More informationChapter 4 Strain and Material Relations
CIVL 222 STRENGTH OF MATERIALS Chapter 4 Strain and Material Relations Terminology 1. Displacement 2. Deformation 3. Strain 4. Average Axial Strain 5. Shearing Strain 6. Poisson s Ratio 7. Mechanical Properties
More informationCREEP AND CREEPRUPTURE BEHAVIOUR OF STRUCTURAL COMPOSITE LUMBER EVALUATED IN ACCORDANCE WITH ASTM D Borjen Yeh T G Williamson
CIBW18/412 INTERNATIONAL COUNCIL FOR RESEARCH AND INNOVATION IN BUILDING AND CONSTRUCTION WORKING COMMISSION W18  TIMBER STRUCTURES CREEP AND CREEPRUPTURE BEHAVIOUR OF STRUCTURAL COMPOSITE LUMBER
More informationFire Engineering Research  Key Issues for the Future II Naples, Italy, 6 9 June Contents
Fire Engineering Research  Key Issues for the Future II Naples, Italy, 6 9 June 013 Contents (State of the art) PhD planning PhD: BEHAVIOUR OF COLDFORMED STEEL BEAMCOLUMNS IN CASE OF FIRE Motivation
More informationStatics and Mechanics of Materials
Statics and Mechanics of Materials Chapter 41 Internal force, normal and shearing Stress Outlines Internal Forces  cutting plane Result of mutual attraction (or repulsion) between molecules on both
More informationMECHANICS OF SOLIDS  BEAMS TUTORIAL 2 SHEAR FORCE AND BENDING MOMENTS IN BEAMS
MECHANICS OF SOLIDS  BEAMS TUTORIAL 2 SHEAR FORCE AND BENDING MOMENTS IN BEAMS This is the second tutorial on bending of beams. You should judge your progress by completing the self assessment exercises.
More informationOverview of Topics. StressStrain Behavior in Concrete. Elastic Behavior. NonLinear Inelastic Behavior. Stress Distribution.
StressStrain Behavior in Concrete Overview of Topics EARLY AGE CONCRETE Plastic shrinkage shrinkage strain associated with early moisture loss Thermal shrinkage shrinkage strain associated with cooling
More informationME 215 Engineering Materials I
ME 215 Engineering Materials I Chapter 3 Properties in Tension and Compression (Part III) Mechanical Engineering University of Gaziantep Dr. A. Tolga Bozdana www.gantep.edu.tr/~bozdana True Stress and
More informationPunching shear behavior of steelconcrete composite decks with different shear connectors
Punching shear behavior of steelconcrete composite decks with different shear connectors *XiaoQing Xu 1) and YuQing Liu 2) 1), 2) Department of Bridge Engineering, Tongji University, Shanghai 200092,
More informationChapter14 CALCULATION OF SECTIONS IN ELASTOPLASTIC DOMAIN
Chapter14 CALCULATION OF SECTIONS IN ELASTOPLASTIC DOMAIN 14.1 GENERALS In all strength calculations made until now, it was used the hypothesis of the linear elastic material, where Hooke s law is valid
More informationFLEXURAL PERFORMANCE OF RC BEAMS STRENGTHENED WITH PRESTRESSED CFRP SHEETS
FLEXURAL PERFORMANCE OF RC BEAMS STRENGTHENED WITH PRESTRESSED CFRP SHEETS Piyong Yu, Pedro F. Silva, Antonio Nanni Center for Infrastructure and Engineering Studies Department of Civil, Architectural,
More informationShear Reinforcements in the Reinforced Concrete Beams
American Journal of Engineering Research (AJER) eissn : 23200847 pissn : 23200936 Volume02, Issue10, pp191199 www.ajer.org Research Paper Open Access Shear Reinforcements in the Reinforced Concrete
More informationANALYSIS FOR BEHAVIOR AND ULTIMATE STRENGTH OF CONCRETE CORBELS WITH HYBRID REINFORCEMENT
International Journal of Civil Engineering and Technology (IJCIET) Volume 6, Issue 10, Oct 2015, pp. 2535 Article ID: IJCIET_06_10_003 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=6&itype=10
More informationUniaxial Tension and Compression Testing of Materials. Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng
Uniaxial Tension and Compression Testing of Materials Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng 3.032 Lab Report September 25, 2013 I. Introduction Understanding material mechanics
More informationFatigue :Failure under fluctuating / cyclic stress
Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue
More informationSimple design method
method Aim of the design method 2 3 Content of presentation in a fire situation method of reinforced concrete slabs at 20 C Floor slab model Failure modes method of at Extension to fire behaviour Membrane
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More informationMECHANICS OF MATERIALS
2009 The McGrawHill Companies, Inc. All rights reserved. Fifth SI Edition CHAPTER 4 MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf David F. Mazurek Pure Bending Lecture
More informationMAE 20 Winter 2011 Assignment 5
MAE 20 Winter 2011 Assignment 5 6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa (16.7 10 6 psi). (a) What is the
More informationLap Shear Tests of Bolted and Screwed Ferritic Stainless Steel Connections. A. Talja, M. Torkar
Lap Shear Tests of Bolted and Screwed Ferritic Stainless Steel Connections A. Talja, M. Torkar VTT, Technical Research Centre of Finland. IMT, Institute of Metals and Technology, Ljubljana, Slovenia Abstract
More informationEXPERIMENTAL INVESTIGATION ON EPOXY BONDED SHEAR CONNECTION FOR TIMBERCONCRETE COMPOSITES
EXPERIMENTAL INVESTIGATION ON EPOXY BONDED SHEAR CONNECTION FOR TIMBERCONCRETE COMPOSITES Rijun Shrestha, James Mak, Keith Crews ABSTRACT: This paper presents the results of an experimental investigation
More informationCHAPTER MECHANICS OF MATERIALS
CHPTER 4 Pure MECHNCS OF MTERLS Bending Pure Bending Pure Bending Other Loading Tpes Smmetric Member in Pure Bending Bending Deformations Strain Due to Bending Stress Due to Bending Beam Section Properties
More informationGLUED TIMBERCONCRETE BEAMS ANALYTICAL AND NUMERICAL MODELS FOR ASSESSMENT OF COMPOSITE ACTION
Engineering Review Vol. Issue 9. GLUED TIMBERCONCRETE BEAMS ANALYTICAL AND NUMERICAL MODELS FOR ASSESSMENT OF COMPOSITE ACTION L. Škec A. Bjelanović * G. Jelenić Faculty of Civil Engineering University
More informationOptimum proportions for the design of suspension bridge
Journal of Civil Engineering (IEB), 34 (1) (26) 114 Optimum proportions for the design of suspension bridge Tanvir Manzur and Alamgir Habib Department of Civil Engineering Bangladesh University of Engineering
More informationSeismic analysis of a 2storey log house Jorge M. Branco a, Paulo B. Lourenço b, Chrysl A. Aranha c
Seismic analysis of a 2storey log house Jorge M. Branco a, Paulo B. Lourenço b, Chrysl A. Aranha c ISISE, Department of Civil Engineering, University of Minho, Guimarães, Portugal a jbranco@civil.uminho.pt,
More informationExperimental evaluation of stone masonry walls with lime based mortar under vertical loads
Structural Repairs and Maintenance of Heritage Architecture XII 401 Experimental evaluation of stone masonry walls with lime based mortar under vertical loads M. AbdelMooty 1, A. Al Attar 2 & M. El Tahawy
More informationPlastic Behaviour  Tensile Strength
Plastic Behaviour  Tensile Strength Transition of mechanical behaviour from elastic to plastic depends upon the material type and its condition as tested (hotrolled, coldrolled, heat treated, etc.).
More informationMATERIALS SELECTION FOR SPECIFIC USE
MATERIALS SELECTION FOR SPECIFIC USE1 Subtopics 1 Density What determines density and stiffness? Material properties chart Design problems LOADING 2 STRENGTH AND STIFFNESS Stress is applied to a material
More informationGrading of the basic material. H. Unterwieser
Grading of the basic material H. Unterwieser Graz, 29. Juni 2007 Content Introduction Standardisation Visual and machine strength grading Presentation of accomplished projects 2 Introduction Why grading
More informationHome Browse Search My settings My alerts Shopping cart
Home Browse Search My settings My alerts Shopping cart Articles All fields Author Images Journal/Book title Volume Issue Page Se Thumbnails FullSize images View View Page 2 of 11 2. Formulation of the
More informationThe University of Bradford Institutional Repository
The University of Bradford Institutional Repository http://bradscholars.brad.ac.uk This work is made available online in accordance with publisher policies. Please refer to the repository record for this
More informationCH 6: Fatigue Failure Resulting from Variable Loading
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
More informationSTRUCTURAL PERFORMANCE OF MANGROVE REINFORCED CONCRETE BEAMS
STRUCTURAL PERFORMANCE OF MANGROVE REINFORCED CONCRETE BEAMS Kallenama Azé Kerté 1, Timothy Nyomboi 2 and Walter Oyawa 3 1 Department of Civil Engineering, Pan African University, Institute for Basic Science,
More informationStructural fire design Eurocode 51.2 Timber structures
Background and Applications Brussels, 1820 February 2008 Dissemination of information workshop 1 Structural fire design Eurocode 51.2 Timber structures Jochen Fornather Austrian Standards Institute jochen.fornather@onnorm.at
More informationAdam Zaborski handouts for Afghans
Tensile test Adam Zaborski handouts for Afghans Outline Tensile test purpose Universal testing machines and test specimens Stressstrain diagram Mild steel : proportional stage, elastic limit, yielding
More informationTHE DETERMINATION OF DELAMINATION STRAIN ENERGY RELEASE RATE OF COMPOSITE BIMATERIAL INTERFACE
THE DETERMINATION OF DELAMINATION STRAIN ENERGY RELEASE RATE OF COMPOSITE BIMATERIAL INTERFACE Jaroslav Juracka, Vladimir Matejak Brno University of Technology, Institute of Aerospace Engineering juracka@fme.vutbr.cz;
More informationTHE STUDY OF LATERAL TORSIONAL BUCKLING BEHAVIOUR OF BEAM WITH TRAPEZOID WEB STEEL SECTION BY EXPERIMENTAL AND FINITE ELEMENT ANALYSIS
THE STUDY OF LATERAL TORSIONAL BUCKLING BEHAVIOUR OF BEAM WITH TRAPEZOID WEB STEEL SECTION BY EXPERIMENTAL AND FINITE ELEMENT ANALYSIS Fatimah Denan 1, Mohd Hanim Osman 2 & Sariffuddin Saad 3 1 School
More informationStudy on Behaviour of Bolted Coldformed Steel Angle Tension Members
Indian Journal of Science and Technology, Vol 8(S7), 102 109, April 2015 ISSN (Print) : 09746846 ISSN (On) : 09745645 Study on Behaviour of Bolted Coldformed Steel Angle Tension Members R. Padma Priya
More informationCOMPARISON OF TIMBER STRENGTH CLASSIFICATION SYSTEMS IN FINLAND AND IN RUSSIA
Saimaa University of Applied Sciences Technology, Lappeenranta Double Degree Programme Civil and Construction Engineering Anastasia Gruznova COMPARISON OF TIMBER STRENGTH CLASSIFICATION SYSTEMS IN FINLAND
More informationLab for Deflection and Moment of Inertia
Deflection and Moment of Inertia Subject Area(s) Associated Unit Lesson Title Physics Wind Effects on Model Building Lab for Deflection and Moment of Inertia Grade Level (1112) Part # 2 of 3 Lesson #
More informationReinforced Concrete Design to BS8110 Structural Design 1 Lesson 5
Lesson 5: Deflection in reinforced concrete beams Content 4.1 Introduction 4. Definitions 4..1 Tension 4.. Compression 4.3 Initial sizing 4.3.1 Worked example 4.4 Reinforcement details 4.5 Anchorage at
More informationEML 5526 FEA Project 1 Alexander, Dylan. Project 1 Finite Element Analysis and Design of a Plane Truss
Problem Statement: Project 1 Finite Element Analysis and Design of a Plane Truss The plane truss in Figure 1 is analyzed using finite element analysis (FEA) for three load cases: A) Axial load: 10,000
More informationBehavior of high strength structural steel at elevated temperatures
University of Wollongong Research Online Faculty of Engineering  Papers (Archive) Faculty of Engineering and Information Sciences 2006 Behavior of high strength structural steel at elevated temperatures
More informationThe elements used in commercial codes can be classified in two basic categories:
CHAPTER 3 Truss Element 3.1 Introduction The single most important concept in understanding FEA, is the basic understanding of various finite elements that we employ in an analysis. Elements are used for
More informationSupplement No. 13 to the Southern Pine Inspection Bureau Grading Rules 2002 Edition
Supplement 3 to the Southern Pine Inspection Bureau Grading Rules 2002 Edition Effective: June 1, 2013 This supplement makes no changes in Table 4a, Table 5, Table 8a, and the Conversion Factors for Determining
More information